Ultrasmall silicon quantum dots - cml. We report the realization of extremely small single quantum...
Embed Size (px)
Transcript of Ultrasmall silicon quantum dots - cml. We report the realization of extremely small single quantum...
Ultrasmall silicon quantum dots F. A. Zwanenburg,1,a� A. A. van Loon,1 G. A. Steele,1 C. E. W. M. van Rijmenam,1
T. Balder,1 Y. Fang,2 C. M. Lieber,2 and L. P. Kouwenhoven1,b� 1Kavli Institute of Nanoscience, Delft University of Technology, P.O. Box 5046, 2600 GA Delft, The Netherlands 2Department of Chemistry and Chemical Biology, Harvard University, Cambridge, Massachusetts 02138, USA
�Received 6 April 2009; accepted 19 May 2009; published online 29 June 2009�
We report the realization of extremely small single quantum dots in p-type silicon nanowires, defined by Schottky tunnel barriers with Ni and NiSi contacts. Despite their ultrasmall size the NiSi–Si–NiSi nanowire quantum dots readily allow spectroscopy of at least ten consecutive holes, and additionally they display a pronounced excited-state spectrum. The Si channel lengths are visible in scanning electron microscopy images and match the dimensions predicted by a model based on the Poisson equation. The smallest dots ��12 nm� allow identification of the last charge and thus the creation of a single-charge quantum dot. © 2009 American Institute of Physics. �DOI: 10.1063/1.3155854�
The observation of quantum states in silicon devices re- quires small structures because of the relatively high electron and hole effective masses compared to, e.g., InAs or GaAs. Top-down planar silicon devices,1–3 produced by etching bulk materials down to nanometer dimensions, often show structural roughness or dopant fluctuations. The correspond- ing potential fluctuations can result in localization on short length scales, and thus multiple dots connected in series. Nearly all reports so far have been on Si quantum dots greater than 50 nm, e.g., in Si metal oxide semiconductor field effect transistors,4–6 silicon-on-insulator structures,1–3,7
and Si/SiGe heterostructures.8,9 In these three systems ex- cited states have been observed only recently.10–12 Silicon nanowires, on the other hand, naturally provide nanometer scale confinement without etching and have demonstrated clean quantum dot behavior early as 2005.13 The latter in- clude excited-state spectroscopy, spin spectroscopy, and a strong indication of the realization of a single-hole dot. We have continued this work and gained a better understanding of the specific system. This has allowed us to realize the first experimental identification of the first four spin states in a silicon quantum dot.14 Here we present a thorough investiga- tion of the Si nanowire quantum dot system and the tech- niques for achieving a single-hole Si nanowire quantum dot, crucial for those results.
We have measured many single quantum dots in p-type silicon nanowires, defined by Schottky tunnel barriers with Ni and NiSi leads. Tunnel barriers defined by Schottky con- tacts remain fairly constant over a large range of dot occu- pation numbers. Gate-defined tunnel barriers, however, are much more sensitive to small shifts in the electrostatic field. Hence the quantum dot regime rapidly changes from weakly coupled to strongly coupled, making it nearly impossible to
observe quantum states. We have realized quantum dots shorter than 30 nm, on which we are able to perform spec- troscopy of at least ten consecutive holes with pronounced excited states. We can make a reliable estimate of the dot length by comparing the measured backgate capacitance to the capacitance computed with a model based on the Poisson equation. The Si channel lengths visible in scanning electron microscopy �SEM� images match the dimensions predicted by the model. Finally, we emphasize the difficulty of creating a single-hole silicon quantum dot, since many single dots split up in two dots upon reaching the few-hole regime. In our experience only very short dots ��12 nm� have allowed identification of the last charge in transport measurements.
II. TWO TYPES OF SI NANOWIRE QUANTUM DOTS
In this section two approaches for fixing the Si channel length are compared: �i� Si nanowires with evaporated Ni contacts which are defined by electron-beam lithography and �ii� NiSi–Si–NiSi nanowires, fabricated by thermally induced diffusion of Ni into Si nanowires. Single-crystal p-type Si nanowires are prepared by a gold nanocluster mediated vapor-liquid-solid process15 using silane and diborane as pre- cursor gases with an atomic feed-in ratio of Si:B=4000:1. The typical diameter is 7–12 nm, comprising a Si core of 3–8 nm and a native oxide of �2 nm. After growth we deposit the nanowires on a highly doped silicon substrate capped with a dry thermal oxide. Predeposited markers allow locat- ing individual nanowires with a SEM and defining contacts by means of electron-beam lithography. The samples are treated with buffered hydrofluoric acid for 5 s prior to metal deposition to etch off the native SiO2. We deposit Ni con- tacts, leaving a Si channel of 50–300 nm uncovered, see Fig. 1�a�. In order to make NiSi–Si–NiSi nanowires the samples are annealed in sequential steps of 20–30 s at 380 and 410 °C to induce radial and longitudinal diffusion of Ni into the Si nanowire. From both Ni contacts a NiSi segment is formed in the nanowires with lengths of 100–150 nm de-
a�Electronic mail: firstname.lastname@example.org. b�Author to whom correspondence should be addressed. Electronic mail:
JOURNAL OF APPLIED PHYSICS 105, 124314 �2009�
0021-8979/2009/105�12�/124314/5/$25.00 © 2009 American Institute of Physics105, 124314-1
Downloaded 13 Aug 2009 to 22.214.171.124. Redistribution subject to AIP license or copyright; see http://jap.aip.org/jap/copyright.jsp
pending on diameter, temperature, and time. The remaining Si section is connected to the lithographically defined Ni contacts by two NiSi leads, see Fig. 1�b�. These devices have room-temperature resistances varying from 100 k� to 5 M�. Some nanowires are fully transformed into the metal NiSi having room-temperature resistances of 1–5 k�, cor- responding to ��10 �� cm, consistent with values found in NiSi nanowires16 and large single crystals.17
III. SINGLE QUANTUM DOTS OF VARYING LENGTHS
The Ni–Si or NiSi–Si interfaces in each device form the Schottky tunnel contacts between the metallic leads and the p-Si quantum dot, see Fig. 1�c�. We have measured 6 Ni– Si–Ni and 30 NiSi–Si–NiSi single quantum dots on sub- strates with SiO2 thicknesses of 50 and 285 nm. They are cooled down to cryogenic temperatures with a pumped 4He cryostat or a dilution refrigerator. Electrical characterization is carried out by measuring the current from drain to ground while sweeping the bias voltage at the source, VSD, and step- ping the backgate voltage, VBG. In Fig. 2 the differential conductance, dI /dVSD, of four devices of varying sizes is plotted versus VSD and VBG. We will refer to devices A-Ni, B-NiSi, C-Ni, and D-NiSi for the respective figures Figs. 2�a�–2�d�.
All four subfigures display diamond-shaped regions in which the current is zero due to Coulomb blockade and the number of holes on the quantum dot, N, is fixed. From these Coulomb diamonds we have derived the most important pa- rameters in Table I. In the smallest diamonds the charging energy EC is equal to the addition energy Eadd. The latter is taken from the height of a Coulomb diamond, indicated as �VSD in Fig. 2�b�. The backgate-to-dot capacitance CBG is calculated as CBG=e /�VBG, where �VBG is the voltage needed to add a single charge, see Fig. 2�b�. The diamond edges have slopes of −CBG /CS and CBG / �C−CS�, where CS �CD� is the capacitance between the dot and source �drain�.
C is the sum of all capacitances to the dot and follows from the charging energy as e2 /C. If we assume that no other gates have a significant capacitive coupling to the dot, then C=CS+CD+CBG. We also compute the gate coupling factor
� as Eadd /�VBG. The length L of the NiSi–Si–NiSi quantum dots is estimated by means of a capacitance model, see Sec. IV. We approximate the number of charges in these Coulomb diamonds by counting up holes from zero, starting at the backgate voltage at which the dot is emptied at a high volt- age bias.
We start by comparing the low temperature measure- ments on the Ni–Si–Ni quantum dot A-Ni and the NiSi–Si– NiSi nanowire quantum dot B-NiSi. Both stability diagrams in Figs. 2�a� and 2�b� display a set of uniform Coulomb diamonds. Besides a longer Si channel, device A-Ni also has a diameter of �20 nm, versus �6 nm for device B-NiSi. The source and drain capacitances of device A-Ni are about ten times bigger than those of device B-NiSi, because of the order of magnitude difference in volume. Naively, one would expect the same ratio for the backgate capacitances, but they have comparable values. The difference in volume is com- pensated by the fact that in a NiSi–Si–NiSi nanowire the leads and quantum dot have comparable diameters, and by the difference in SiO2 thickness. The first strongly reduces screening of the backgate compared to lithographically de- fined leads of device A-Ni.
Outside the diamonds of device B-NiSi many lines of increased conductance run parallel to the edges, whereas the conductance of device A-Ni shows no such structure. The origin can be found in the availability of extra channels for transport. Lines ending on the Nth diamond are attributed to
SiNiSiNi NiSi Ni
FIG. 1. �Color� Two types of Si nanowire quantum dots. Schematic top view of a Si nanowire quantum dot �a�